1 Corrosion of Steel, Aluminum and Copper in Electrical Applications By: Alex Mak, P. Eng. - Senior Field Applications Engineer, General Cable Executive Summary Corrosion, typically defined as the deterioration of metals through the combined actions of oxygen, other metals and salts, has a major impact on industrial economies. But despite the damage it does, and the seriousness of the issue in economic terms, awareness of ways corrosion can be controlled is in surprisingly short supply. In the United States, Japan, Great Britain and Australia, studies of the economics of corrosion have indicated that its cost to the economy runs in the vicinity of 3-4 per cent of Gross National Product. Further, in a world where businesses are looking for ways to simultaneously stretch budgets and address concerns about the sustainability of their processes, corrosion presents another problem. Of the new steel consumed every year around the world, it is estimated that roughly 20 per cent is used to replace metal lost to corrosion1. As is often the case, the reality on the ground is a lot messier than the scientific explanation. In theory, corrosion processes are easy to describe, but the truth of the matter is that corrosion is a multi-phased process that can sometimes result in secondary chemical agents that are as damaging as the corrosion itself. Hydrogen evolution is a good example of this. While corrosion is the main culprit, the resultant processes further weaken metallic components. Likewise, the corrosion resistance properties of various metals often thought of as a cut-and-dry matter are much more complex than they appear at first glance. Considering the cost it exacts on our economy, it is surprising that corrosion is such a misunderstood process, and that it is often treated as an uncontrollable cost of doing business. By acquiring knowledge of the corrosion process, we can better understand how to limit its negative effects. This paper provides a brief overview of corrosion and explores how best to control it by examining its impact on the three most commonly used metals in electrical installations: copper, steel and aluminum. Why Metals Corrode To reduce it to simplest possible terms, corrosion is really nothing more than the inherent tendency of metals to revert from a processed, metallic state to their more natural state, which we commonly call ore. Most metals, with the exception of precious metals, such as gold and platinum, do not occur in metal form in nature they exist as ore. When ore is processed into metal, the refining process transfers its latent energy to the ore. It is the taking on of this latent energy that transforms ore into metal, but by taking on this energy, the metal elevates to a higher energy state, which means it also becomes less thermodynamically stable. Corrosion is really nothing more than the inherent tendency of metals to revert from a processed, metallic state to their more natural ore state. The process of metal, in its new high-energy state, reverting to its lower energy (ore) state is what we call corrosion. It is, quite simply, the means by which metal returns to its more stable, lower energy mineral state through the release of the latent energy acquired in refinement. Precious metals such as gold and platinum exist naturally in their metal state and have intrinsic thermodynamic stability. All other metals are prone to corrosion. In some cases, metals can form oxide films as part of the corrosion process. Some metals form oxide films that are porous while other metals form oxide films that buckle and flake off. In both cases, the underlying metal is subject to continued oxidation process and results in metal loss. But there can be an upside to oxide films as well. Metals that form a tightly adhering layer of surface oxides are much more corrosion resistant because the adhering layer known as the passivation layer - offers significant protection by isolating the metal from the corrosive environment. How Corrosion Works Four conditions must exist for corrosion to occur: There must be an anode (corroding) and a cathode 1Vander Velde, H Corrosion Testing and Rehabilitation of Unbonded post tensioned cables in Push-Through or Heat Sealed Sheaths, In Seminar on Parking Garages, Toronto, Edited 2002.
2 (protected) component There must be an electrical potential between the anode and the cathode The anode and cathode must be immersed in an electrolyte, which is an electrically conductive fluid The anode and cathode must be connected by a metal path of low resistance In other words, corrosion is essentially an electrical circuit wherein electrons flow from the anode to the cathode. When electrons flow from the anode, the anode oxidizes to form metallic ions. These metallic ions then detach from the metal surface to flow toward the cathode through the electrolyte. Throughout this process the metallic ions may also react with elements in the electrolyte to form other compounds. Rust is a good example. Rust (also known as FeOOH) is created when iron ions react with various elements in the water. As the electrons flow across the low-resistance metallic path to the cathode, the cathode is reduced and the formation of metal ions is halted. When the metal is not in a positively charged ionized form, it is much less reactive. This is why the cathode develops an inherent protection from metal loss to corrosion. Below is an example (Figure 1) showing how iron is oxidated (loses electrons and becomes a metallic ion) and reacts with the hydroxide irons present in the electrolyte, thus forming FeOOH (rust). Oxygen is frequently involved in the corrosion process because most metals in ore form are typically oxides. For example, iron and aluminum exist in nature as an oxide (Al 2 and Fe 2 respectively). Copper, on the other hand, is typically found as copper sulfate. This means that in the presence of sulfur, copper will readily react with sulfur to return back to its natural state of copper sulfate. The Electrical Metals: Steel, Aluminum and Copper Steel, aluminum and copper are the three main metals used in electrical applications. Steel is typically used in housing, enclosure and support systems (struts and cable trays). Copper is often used in conductors. And aluminum can be found most often in conductors, conduits, armor and supports (cable trays). Each of these metals is susceptible to corrosion and there are many misconceptions about the corrosion resistance of each. The electrical industry generally considers copper to be corrosion resistant in virtually all environments while regarding steel and aluminum as non-resistant. However, this is an over-generalization. Of the three metals copper is the most cathodic, or noble, and is typically less affected by galvanic reactions. As a result, the electrical industry generally considers copper to be corrosion resistant in virtually all environments while regarding steel and aluminum as non-resistant. However, this is an overgeneralization in what should be thought of in more relative terms. The truth of the matter is that copper tends to get a free ride at the expense of other metals. Were it to be used in contact with more noble metals such as passive nickel, passive stainless 316 and 304 stainless steel or titanium, copper would galvanically deplete just as readily as steel or aluminum do. Atmospheric, Soil and Galvanic Corrosion In general, atmospheric, soil and galvanic corrosion represent the major types of corrosion metals are exposed to in the electrical industry. Atmospheric Corrosion of Steel Steel typically corrodes or rusts rapidly in moist environments, and the rate of corrosion accelerates with exposure to salt water. As mentioned previously, Fe 2 forms on the surface of iron or steel to act as a passivating layer. However, in the presence of water, oxygen, and sulfur dioxide and carbon dioxide solutions, the protective Fe 2 layer becomes non-protective rust (FeOOH) due to the formation of Fe 3 O 4. Figure 1 This layer is continually flaking off at the surface to expose fresh metal to corrosion. This process carries on until either all of the iron or all of the oxygen, water, carbon dioxide, or sulfur dioxide in the system is removed or consumed In electrical applications where steel is usually used as the housing, enclosure or support system material, corrosion needs to be controlled by measures such as galvanizing, alloying, or painting. Galvanizing steel with zinc provides steel with a sacrificial anode that will continually deplete to protect the
3 more cathodic steel. Alloying steel with chromium allows for the formation of a tightly adhering surface oxide layer, thus turning steel into stainless steel. Painting prevents corrosion by sealing out the agents of corrosion listed above. Atmospheric Corrosion of Copper Copper can sometimes be found naturally in a metal state and is therefore thermodynamically stable in most atmospheric conditions. As a result, copper is widely used for roofing and other applications where it will come into contact with water. Copper develops a strongly adhering oxide layer, which thickens to acquire the familiar green patina we see on copper roofs. In the presence of atmospheric sulfur dioxide (SO 2 ) the transition from oxide layer to patina is accelerated. In applications such as roofing where the green patina has aesthetic value, the increase in formation of patina is desirable. This is definitely not the case in electrical system applications where the formation of this thick non-conductive patina is undesirable. Where the greenish corrosion product is found on a copper conductor, this corrosion product must be removed by means of a wire brush or emery cloth to ensure low resistance contact between conductor and connector. Atmospheric Corrosion of Aluminum Only beryllium, potassium, sodium and magnesium are more thermodynamically reactive than aluminum. However, a signature property of aluminum is its tendency to form a strongly bonded passivating oxide film on its surface. For this reason, it offers excellent resistance to corrosion and provides years of maintenance-free service in natural atmospheres. At an ambient temperature of 25 degrees C, the normal surface film formation is only about 2-50nm thick. If damaged by a fresh abrasion for example this corrosion-protective film re-forms immediately in most environments and ensures continued protection. As a result, aluminum and its alloys are used in a wide range of applications that include buildings, power lines, large ship superstructures, truck transports, railroad and subway cars, water pipelines, beverage containers (soft drink and beer cans), and chemical industry tanks, piping, barges, reaction vessels, and distillation columns2. In applications where exposure to the elements particularly water is a factor, you can be sure you will find aluminum being used. For an excellent example of aluminum s time-proven resistance to corrosion at work in the electrical industry, look no further than bare aluminum transmission conductors, which have been hard at work and resisting corrosion now for over 100 years. Soil Corrosion of Steel The reaction of carbon steel to soil corrosion depends primarily on the composition of the soil and other environmental factors, including the presence and abundance of moisture and oxygen. The extreme variability of these factors amounts to extreme variation in the rate of attack by corrosion. Consider, for instance, that a buried iron vessel in the worst possible soil conditions may perforate in less than a year, and yet iron tools hundreds of years old have been unearthed by archeologists in arid dessert regions. As a rule, soils with high moisture content, high electrical conductivity, high acidity, and high dissolved-salt content will be most corrosive3. For this reason, exposed steel is not often buried in the ground in electrical applications, and as a result, soil corrosion of steel is rarely a concern. Soil Corrosion of Copper A relatively noble metal, copper forms the passivating protective layer that has been referenced previously. In this case the layer is a reddish-brown film, otherwise known as cuprous oxide (Cu 2 0). In most cases, the protective film on copper remains intact or is readily repaired under most soil conditions. But there are situations that will destroy the protective layer and prevent its renewal, causing copper to become susceptible to corrosion in certain soils. Aggressive copper corrosion scenarios can be expected where: There is a combination of elevated sulfate or chloride content and water content resulting from poor drainage, high soil capacity for moisture retention or moderate to heavy annual rainfall (usually more than 76 cm [30in.]). While elevated concentrations of sulfate, chloride, or both in the soil are probably the primary factor in underground corrosion of copper, considerable moisture must be present to support the electrochemical activity required. The sulfates and chlorides may not adversely affect the copper if rainfall is slight and drainage is adequate. There is very low soil resistivity (less than ohmcm). There are large quantities of organic matter (particularly soils containing organic acids). Cinder fills are present, either because of the sulfides present, or because of the galvanic action created by the carbon particles in the cinders. Copper is anodic to carbon, and corrosion should be expected if the cinders used for backfill contain appreciable amounts of carbon. Moisture must be present for the required galvanic action to take place. 2Corrosion of Aluminum and Aluminum Alloys, Edited by Joseph R. Davis, Conditions Contributing to Underground Copper Corrosion, Edited by J.R. Myers and A. Cohen, Source: Copper.org.
4 There are active anaerobic bacteria (sulfate-reducing species) that can produce sulfides. There are inorganic acids. There are soils containing appreciable amounts of ammonia compounds, which are usually corrosive to copper4. Another handy rule of thumb: clay sand, gravel, loam, and chalk seldom possess the combination of properties that promote corrosion of copper in soil. In electrical applications, where bare copper is commonly used for electrical grounding rings and electrodes, special attention needs to be paid to soil conditions. Soil Corrosion of Aluminum According to the US Army Corps of Engineers, Aluminum has excellent corrosion resistance in a wide range of water and soil conditions because of the tough oxide film that forms on its surface. Although aluminum is an active metal in the galvanic series, the oxide film affords excellent protection except in several special cases. While it is true that aluminum s protective oxide film is stable in a ph range from 4.5 to 8.5, the cocktail of compounds present is crucial. Certain soils tend to be more corrosive to aluminum, particularly non-draining clay-organic mucks. As a general rule, contact with clay soils should be minimized unless special corrosion treatment measures are instituted. 4 It is for this reason that the National Electric Code and the Canadian Electric Code ban the use of bare aluminum in soil. Galvanic Corrosion of Steel, Copper and Aluminum Galvanic corrosion is probably the leading cause of all corrosion experienced by steel and aluminum in electrical applications. Unlike structural or mechanical applications where metals can be electrically insulated, electrical applications require direct metal-to-metal contact. Galvanic corrosion occurs when two metals of different potentials come into direct contact with one another while immersed in an electrolyte. The two metals difference in potential causes current to flow from the cathode to the anode, which, as we have seen, leads to oxidation of the anode and reduction of the cathode. As described previously, this results in the corrosion of the anode and the protection of the cathode from corrosion. Figure 1 below shows the potential difference measured between various metals and the standard hydrogen electrode. Electrode Potential Element (Volts) Lithium Rubidium Potassium Calcium Barium Sodium Magnesium Aluminum Zinc Chromium Iron Nickel Tin Lead Hydrogen Copper Iodine Silver Gold Mercury Iodide Bromine Chlorine Fluorine Figure 1: Electrode potential of various metals versus the standard hydrogen electrode. Copper, which we have seen to be a relatively noble metal, does not usually exhibit a great deal of galvanic corrosion. However, in cases where bare copper is buried in soil with high cinder fill content, the carbon in the cinder fill will cause the copper to become anodic and corrosion to occur. Due to its position in the galvanic series, steel is prone to galvanic corrosion. This is not typically an issue in electrical applications because steel components are not usually required to be electrically conductive. This means they can be insulated from the other metals to eliminate the metal-to-metal contact corrosion requires. For aluminum, due to its inherent resistance to other forms of corrosion, the galvanic process is the most common cause of corrosion. When aluminum, a reactive metal in the galvanic series, comes into contact with other more cathodic metals, it acts as a sacrificial anode and becomes susceptible to corrosion. Understanding galvanic corrosion has lead to the use of metals 4United States Army Corps of Engineers, EM Design of Seawalls and Bullheads. Washington, DC: USACE, 1995.
5 in the galvanic series for cathodic protection. For example, electrically connecting buried steel pipe with zinc, which is more anodic, allows the zinc to corrode before the steel. It is offered up as a sacrificial anode and limits the corrosion of the steel pipe until all of the zinc is consumed. Preventative Measures Atmospheric Corrosion When steel is used for housing and structural components, it is chosen for its cost and strength. For all its benefits, it is relatively susceptible to atmospheric corrosion. Coating or painting is required to separate the steel from the water and other agents that facilitate the corrosive process. Millions of automobiles are a testament to the effectiveness of this approach. Copper, which is highly noble, is well known as a suitable metal for most atmospheric applications. However, in locations with elevated sulfur (such as H 2 S) and ammonia content, use of copper should be avoided. When copper conductors are used in these environments, special oxide inhibiting pastes need to be applied. This is the reason why nickel-plating and tin-plating are also widely used as means to prevent copper corrosion. When working with copper, care must also be taken to remove the thickened oxide layer (patina), as this layer is non-conductive and will degrade the integrity of the electrical circuit. Aluminum is typically corrosion resistant in most atmospheric conditions, and unlike copper, it does not corrode in sulfur or ammonia rich environments. However, it is also important to remember that aluminum is vulnerable to galvanic corrosion. Soil Corrosion As discussed earlier, soil corrosion is normally not a major concern for steel in electrical applications. Due to its cathodic nature, copper is the standard conductor for use in grounding electrodes and grounding rings. In order to eliminate the possibility of galvanic corrosion of copper caused by carbon content, care must be taken to ensure cinder fill is not present in areas where copper is being used. Care should also be taken to insulate underground steel pipes when grounding them to copper grounding conductors in order to prevent galvanic corrosion of the steel. ranging from ph. Galvanic Corrosion Unless exposed to high carbon content (cinder fill), galvanic corrosion does not usually arise as an issue for copper due to the noble nature of the metal. Steel, less noble than copper, will corrode when the two metals are in contact with one another. Wherever possible, these two metals should be insulated from each other. In situations where direct contact is required such as copper bonding conductors connecting to steel enclosures, an oxide-inhibiting paste should be applied. This will keep moisture (electrolyte) away from the contact area and limit the potential for a galvanic reaction between the two metals. Aluminum is the most reactive metal among the three metals discussed. As a result, galvanic corrosion is the most commonly occurring form of corrosion in aluminum electrical applications. Often used as an electrical conductor in either cable form, connector form or as the bussing in panels, aluminum will require tin-plated bussing and connectors to mitigate galvanic reaction when connected to copper or steel. An oxide-inhibiting compound should also be used to ensure moisture (electrolyte) does not reach the contact surface and facilitate galvanic reaction. The best way to eliminate galvanic corrosion is to: Select metals that are close together in the galvanic series Isolate the metals from each other using insulating materials Eliminate the presence of electrolyte on the metal surface Maintain a large surface anodic area in relation to the cathodic area Conclusion Understanding the corrosion process will help in reducing the safety and economic impact of corrosion damage. As discussed in this paper, each metal used is subject to its own unique corrosion process. Aluminum and copper are both widely used conductor materials and each has its own benefits. The metal selected for each application needs to have the necessary mechanical, electrical and chemical properties to fulfill its intended function, while meeting the economic requirements of the installation. Generally speaking, aluminum in electrical applications is not permitted for use in direct contact with soil, and aluminum conductors are insulated to eliminate possible corrosion due to extreme soil ph levels outside of aluminum s safe range. Aluminum is considered to be corrosion resistant in soils
Dr. Ali Abadi Chapter 5: Chemical Effect Materials Properties (Corrosion) Introduction 1 By the end of this tutorial, you should have an understanding of: relative susceptibility of different metals to
A SHORT INTRODUCTION TO CORROSION AND ITS CONTROL CORROSION OF METALS AND ITS PREVENTION WHAT IS CORROSION Corrosion is the deterioration of materials by chemical interaction with their environment. The
FUNDAMENTALS OF CATHODIC PROTECTION Corrosion is the deterioration of a metal because of a reaction with its environment. For the purpose of this report, corrosion is the result of an electrochemical reaction
Basics of Corrosion Performance Metals Sacrificial anode manufacturer Specialize in aluminum alloy anodes All products made in the USA (Berks county, PA) ISO9001/2001 Certified Quality System Also traditional
S t r o n a 1 Author: Marta Miedźwiedziew METAL CORROSION AND PROTECTION AGAINST CORROSION Introduction The article is intended for high school students having courses in chemistry at both the basic and
Beginners Guide to Corrosion This document has been prepared by Bill Nimmo and Gareth Hinds of NPL s Corrosion Group from various source material. It is intended to give an introduction to corrosion and
Chemistry 12 UNIT 5 OXIDATION AND REDUCTION PACKAGE #2 HOW TO PREDICT WHETHER A REDOX REACTION WILL BE SPONTANEOUS: Looking at the table in the data booklet on page 8, INCREASING TENDENCY TO REDUCE = INCREASING
Corrosion Control & Cathodic Protection for Water & Wastewater Systems Presented By: James T Lary Corrpro Companies, Inc 1090 Enterprise Dr. Medina, OH 44256 Tel. 330-723 723-5082 (x1215) email: email@example.com
EDEXCEL INTERNATIONAL GCSE CHEMISTRY EDEXCEL CERTIFICATE IN CHEMISTRY ANSWERS SECTION C Chapter 16 1. Burn sulfur in air to give sulfur dioxide. S(s) + O 2 (g) ----> SO 2 (g) Pass this with more air over
35 MOLES ND MOLE CLCULTIONS INTRODUCTION The purpose of this section is to present some methods for calculating both how much of each reactant is used in a chemical reaction, and how much of each product
Corrosion can be defined as the destructive attack of a metal by an electrochemical reaction with its environment. Steel exposed to moisture and oxygen will rust and corrode. Corrosion is defined as the
A PT E R TWELVE SE et ION I 2. I What is corrosion? If you have an old bicycle then you will probably have seen how corrosion can destroy metals. For example, the steel in the cycle chain can slowly turn
Cambridge International Examinations Cambridge International General Certificate of Secondary Education *0123456789* CHEMISTRY 0620/03 Paper 3 Theory (Core) For Examination from 2016 SPECIMEN PAPER 1 hour
Metals and Non-metals Comparison of physical properties of metals and non metals PHYSICAL PROPERTY METALS NON-METALS Physical State Metallic lustre (having a shining surface) Mostly solids (Liquid -mercury)
47374_04_p25-32.qxd 2/9/07 7:50 AM Page 25 4 Atoms and Elements 4.1 a. Cu b. Si c. K d. N e. Fe f. Ba g. Pb h. Sr 4.2 a. O b. Li c. S d. Al e. H f. Ne g. Sn h. Au 4.3 a. carbon b. chlorine c. iodine d.
Science Grade 10-12 Classroom Individual reading DESCRIPTION The characteristic red color of Prince Edward Island soil can be explained by a chemical reaction. The process is known as corrosion or rusting.
Removing Heavy Metals from Wastewater Engineering Research Center Report David M. Ayres Allen P. Davis Paul M. Gietka August 1994 1 2 Removing Heavy Metals From Wastewater Introduction This manual provides
Cathodic Protection Use On Tank Bottoms & Underground Piping In Power Generation Plants PG&E Office San Francisco January 18, 2007 Craig K. Meier Corrosion Control Incorporated Corrosion process for tanks
Electrochemistry Chapter 21a Electrochemistry: The Electrolytic Cell Electrochemical reactions are oxidation-reduction reactions. The two parts of the reaction are physically separated. The oxidation reaction
GCSE CHEMISTRY Higher Tier Chemistry 1H H Specimen 2018 Time allowed: 1 hour 45 minutes Materials For this paper you must have: a ruler a calculator the periodic table (enclosed). Instructions Answer all
Page 1 of 7 These guidelines provide requirements for all University faculty, staff, and students using, handling, or storing combustible metals. These requirements are established to ensure faculty, staff
The position of hydrogen in the reactivity series Hydrogen, although not a metal, is included in the reactivity series because it, like metals, can be displaced from aqueous solution, only this time the
Section 1: are located on the left side of the periodic table and are generally shiny, malleable, ductile, and good conductors. K What I Know W What I Want to Find Out L What I Learned Essential Questions
Introduction Learning Guide 3A Salts Chem 1010 Look at the samples in the two bottles you were given. What observations can you make about them? A: B: If you could look at them more closely, here's what
2009, American Society of Heating, Refrigerating and Air-Conditioning Engineers, Inc. (www.ashrae.org). Published in ASHRAE Journal, Vol. 51, April 2009. This posting is by permission of ASHRAE. Additional
Q. Crude oil is a complex mixture of hydrocarbons, mainly alkanes. The number of carbon atoms in the molecules ranges from to over 00. (a) How does the boiling point change as the number of carbon atoms
D E P A R T M E N T O F M A T E R I A L S S C I E N C E A N D E N G I N E E R I N G M A S S A C H U S E T T S I N S T I T U T E O F T E C H N O L O G Y 3.014 Materials Laboratory Fall 2006 LABORATORY 3:
31 CHEMICAL EQUATIONS and REACTION TYPES The purpose of this laboratory exercise is to develop skills in writing and balancing chemical equations. The relevance of this exercise is illustrated by a series
Ionic and Metallic Bonding BNDING AND INTERACTINS 71 Ions For students using the Foundation edition, assign problems 1, 3 5, 7 12, 14, 15, 18 20 Essential Understanding Ions form when atoms gain or lose
EXPERIMENT #9 CORROSION OF METALS Objective The objective of this experiment is to measure the corrosion rate of two different metals and to show the effectiveness of the use of inhibitors to protect metals
Crevice Corrosion on Stainless Steel Propeller Shafts A Quick Summary: What is it? How to Prevent it. How to Repair it. Stainless steel propeller shafts and running gear are subject to pitting & crevice
7.4 Using the Bohr Theory LEARNING TIP Models such as Figures 1 to 4, on pages 218 and 219, help you visualize scientific explanations. As you examine Figures 1 to 4, look back and forth between the diagrams
Material: laboratory display of the elements and a wall periodic table is required. Objective: To learn the use of periodic table for writing electron configuration of elements. INTRODUCTION Basic building
Equipment Damage Consultants, LLC Fire Event Electronic and Mechanical System Damage Mechanisms Is Acid Gas for Real? Irreparable damage to electronic equipment and mechanical systems away from the actual
Connections Understanding Chemical Equations Have you ever... Seen the result of mixing baking soda and vinegar? Used friction to light a match? Seen a car eaten through by rust? Chemical equations model
Periodic Table Questions 1. The elements characterized as nonmetals are located in the periodic table at the (1) far left; (2) bottom; (3) center; (4) top right. 2. An element that is a liquid at STP is
Oxidation And Degradation Products Of Common Oxygen Scavengers By John D. Zupanovich, ChemTreat, Inc. For many years, sulfite and hydrazine were the principal materials used to protect boiler systems from
Experiment 3 The Electrical Control of Chemical Reactions E3-1 E3-2 The Task In this experiment you will explore the processes of oxidation and reduction, in which electrons flow between materials, and
1. The elements on the Periodic Table are arranged in order of increasing A) atomic mass B) atomic number C) molar mass D) oxidation number 2. Which list of elements consists of a metal, a metalloid, and
Metals and their Uses C Revision (higher) 74 minutes 74 marks Page of 3 Q. The picture shows a diamond ring. Photograph supplied by Comstock/Thinkstock (a) Diamond is a form of carbon. A carbon atom has
90933 909330 1SUPERVISOR S Level 1 Chemistry, 2015 90933 Demonstrate understanding of aspects of selected elements 9.30 a.m. Tuesday 24 November 2015 Credits: Four Achievement Achievement with Merit Achievement
SCH 4C1 Unit 2 Problem Set Questions taken from Frank Mustoe et all, "Chemistry 11", McGraw-Hill Ryerson, 2001 1. A small pin contains 0.0178 mol of iron. How many atoms of iron are in the pin? 2. A sample
UK Aluminium Industry Fact Sheet 2 Aluminium and Corrosion +44(0)121 601 6363 www.alfed.org.uk 1 Introduction Although aluminium is a very reactive metal with a high affinity for oxygen, the metal is highly
The formation of polluted mine water Abandoned Mine Drainage How it happens How we can fix it Bruce Golden Western PA Coalition for Abandoned Mine Reclamation What we ll cover Brief Discussion about Mining
Redox and Electrochemistry This section should be fresh in your minds because we just did this section in the text. Closely related to electrochemistry is redox chemistry. Count on at least one question
Name Writing and Balancing Chemical Equations Period When a substance undergoes a chemical reaction, chemical bonds are broken and new bonds are formed. This results in one or more new substances, often
Page : 1 of 13 Project Engineering Standard www.klmtechgroup.com KLM Technology #03-12 Block Aronia, Jalan Sri Perkasa 2 Taman Tampoi Utama 81200 Johor Bahru Malaysia ELECTIRAL GROUNDING TABLE OF CONTENT
Proceedings of the 32nd International Symposium for Testing and Failure Analysis November 12-16, 2006, Renaissance Austin Hotel, Austin, Texas, USA Accelerated Corrosion of Printed Circuit Boards due to
CHAPTER 1 The Nature of Chemistry Objectives You will be able to do the following. 1. Describe how science in general is done. 2. Given a description of a property of a substance, identify the property
Zirconium in Sulfuric Acid Pickling Applications INTRODUCTION For more than 30 years, zirconium has been successfully used in hot sulfuric acid tanks for pickling steel. Zirconium is uniquely suited for
Chapter 5 Atomic Theory: The Nuclear Model of the Atom Section 5.1 Dalton s Atomic Theory Goal 1 Precursors to John Dalton s atomic theory Law of Definite Composition The percentage by mass of the elements
CHAPTER 3 Metals and Non-metals Multiple Choice Questions 1. Which of the following property is generally not shown by metals? (a) Electrical conduction (b) Sonorous in nature (c) Dullness (d) Ductility
1 CORROSION AND CORROSION PROTECTION A short introduction course by Roy Johnsen, Professor NTNU 2 WHO IS ROY? Siv.ing. NTH 1979 Dr.ing. NTH 1984 Scientist SINTEF 1981-1985 Research Manager Statoil 1985-1991
Chapter 7 Durability and Service Life Lester H. Gabriel, Ph.D., P.E. DURABILITY AND SERVICE LIFE Durability of Drainage Pipes Durability is the property to resist erosion, material degradation and subsequent
St Peter the Apostle High School Chemistry Department Formulae, Equations & Formula Mass N4 & N5 Homework Questions Answer questions as directed by your teacher. National 4 level questions are first followed
EXAMPLE EXERCISE 4.1 Change of Physical State State the term that applies to each of the following changes of physical state: (a) Snow changes from a solid to a liquid. (b) Gasoline changes from a liquid
CHAPTER 5 2 Grouping the Elements SECTION The Periodic Table BEFORE YOU READ After you read this section, you should be able to answer these questions: Why do elements in a group have similar properties?
Instructions for Conversion Problems For every conversion problem Write the number in the problem down with unit and a multiplication sign Decide which conversion factor you should use, Avagadro s or molar
Discovering Electrochemical Cells Part I Electrolytic Cells Many important industrial processes PGCC CHM 102 Cell Construction e e power conductive medium What chemical species would be present in a vessel
Question Bank Electrolysis 1. (a) What do you understand by the terms (i) electrolytes (ii) non-electrolytes? (b) Arrange electrolytes and non-electrolytes from the following substances (i) sugar solution
Cathodic Protection and Interferences René Gregoor Madrid, June 18 th and 19 th 2009 1 Cathodic protection and interferences Corrosion Cathodic protection Protection criterion ON potential measurements
Chemistry Elements, Compounds, subscript, superscript, coefficient Periodic Table o Periods, groups, etc. o Metals o Non-metals o Metalloids The patterns are related to the chemical properties of the element.
CHAPTER 4: MATTER & ENERGY Problems: 1,3,5,7,13,17,19,21,23,25,27,29,31,33,37,41,43,45,47,49,51,53,55,57,59,63,65,67,69,77,79,81,83 4.1 Physical States of Matter Matter: Anything that has mass and occupies
Anodizing Reference Guide Type Thickness Type II Conventional coatings produced 1.8µ-25.4µ from sulfuric acid bath Type I A Conventional coatings produced 0.5µ-7.6µ (microns) from chromic acid bath Type
ATI 316Ti Stainless Steel: Austenitic (UNS S31635) GENERAL PROPERTIES ATI 316Ti stainless is a titanium-stabilized version of Type 316 molybdenum-bearing austenitic stainless steel. It is also known as
Facilities and Campus Services EHS/RMS 3101 Science Circle CPISB Room 102B Anchorage, AK 99508 Oxidizer(s) Management and Use Guidelines This document provides information concerning the handling, storage,
Programme in mole calculation Step 1 Start at the very beginning Atoms are very small indeed! If we draw a line 1 metre long, 6,000,000,000 (6 billion) atoms could be lined end to end. So a scientist cannot
NiMH Batteries for Energy Storage Applications John J.C. Kopera Cobasys Who Is Cobasys? An independently managed 50-50 joint venture to further develop and advance the commercialization of Ovonic Nickel
Oxidation-Reduction Reactions What is an Oxidation-Reduction, or Redox, reaction? Oxidation-reduction reactions, or redox reactions, are technically defined as any chemical reaction in which the oxidation
AP Chem Summer Assignment Worksheet #1 Atomic Structure 1. a) For the ion 39 K +, state how many electrons, how many protons, and how many 19 neutrons are present? b) Which of these particles has the smallest
Instruction manual VWR unstirred water baths Introduction VWR laboratory thermostatic baths provide the means to maintain samples at a precise temperature from just above room temperature up to 99 0 C.
Corrosion of Copper in Water Digby D. Macdonald Center for Electrochemical Science and Technology Department of Materials Science and Engineering Pennsylvania State University 209 Steidle Bldg University
Teacher s Guide Grade Level: 9 12 Curriculum Focus: Chemistry Description Disc 1. Alkali Metals and Alkaline-Earth Metals These elements are highly reactive and rarely found uncombined in nature. The alkaline-earth
Serial Number MODEL 9020 & 9020-OEM CORRATER TRANSMITTER USER MANUAL ROHRBACK COSASCO SYSTEMS, INC. 11841 East Smith Avenue Santa Fe Springs, CA 90670 Tel: (562) 949-0123 (800) 635-6898 Fax: (562) 949-3065
Corrosion If you've ever wondered why prospectors don't find nuggets of aluminium or iron in the wild it's because these metals (among many) can not exist for very long in their refined state. Like most
Chapter 1: Moles and equations 1 Learning outcomes you should be able to: define and use the terms: relative atomic mass, isotopic mass and formula mass based on the 12 C scale perform calculations, including
Periodic Table Instructional Background Patterns in Element Properties (History): Elements vary widely in their properties, but in an orderly way. In 1869, the Russian chemist Dmitri Mendeleev produced
Name: Class: Date: ID: A Chapter 6 Assessment Multiple Choice Identify the choice that best completes the statement or answers the question. 1. When an atom loses an electron, it forms a(n) a. anion. c.
Magnesium TM Soil Anodes High Potential Magnesium SuperMag High Potential Magnesium Anodes from Galvotec Alloys, Inc. offers typical high workingldriving potentials of -1.70 volts or better vs. copperlcopper
Voltaic Cells Introduction In this lab you will first prepare a set of simple standard half-cells and then measure the voltage between the half-cells with a voltmeter. From this data you will be able to
Chapter 2 Atoms Molecules and Ions Student: NOTE: A periodic table is required to work many of the problems in this chapter. 1. The elements in a column of the periodic table are known as A. metalloids.
Balancing Chemical Equations Worksheet Student Instructions 1. Identify the reactants and products and write a word equation. 2. Write the correct chemical formula for each of the reactants and the products.